#------------------------------------------------------------------------------
#$Date: 2016-02-18 17:37:37 +0200 (Thu, 18 Feb 2016) $
#$Revision: 176729 $
#$URL: svn://www.crystallography.net/cod/cif/1/10/10/1101079.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1101079
loop_
_publ_author_name
'Kruger, Hannes'
'Kahlenberg, Volker'
'Kaindl, R.'
_publ_section_title
;
Structural studies on Na6Si8O19 - a monophyllosilicate with a
new type of layered silicate anion
;
_journal_name_full               'Solid State Sciences'
_journal_page_first              1390
_journal_page_last               1396
_journal_paper_doi               10.1016/j.solidstatesciences.2005.08.002
_journal_volume                  7
_journal_year                    2005
_chemical_formula_sum            'Na6 O19 Si8'
_chemical_formula_weight         666.66
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90.00
_cell_angle_beta                 90.140(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   4.9038(5)
_cell_length_b                   23.481(3)
_cell_length_c                   15.392(2)
_cell_measurement_temperature    293(2)
_cell_volume                     1772.3(4)
_diffrn_ambient_temperature      293(2)
_diffrn_source_current           40
_diffrn_source_power             2.00
_diffrn_source_voltage           50
_exptl_crystal_density_diffrn    2.498
_refine_diff_density_rms         0.125
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               1101079
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Si1 Si 0.2017(4) 0.19407(7) -0.36169(12) 0.0158(4) Uani 1 1 d . . .
Si2 Si 0.8047(4) 0.13559(8) -0.08868(12) 0.0161(4) Uani 1 1 d . . .
Si3 Si -0.2091(4) -0.00669(7) -0.35632(12) 0.0155(4) Uani 1 1 d . . .
Si4 Si -0.8027(4) -0.15861(7) -0.32271(12) 0.0156(4) Uani 1 1 d . . .
Si5 Si -0.6996(4) 0.06614(7) -0.32601(12) 0.0154(4) Uani 1 1 d . . .
Si6 Si 0.3025(4) 0.06179(7) -0.12038(12) 0.0153(4) Uani 1 1 d . . .
Si7 Si 0.7039(4) 0.21609(7) -0.24782(12) 0.0154(4) Uani 1 1 d . . .
Si8 Si -0.3025(4) -0.10513(7) -0.23390(12) 0.0158(4) Uani 1 1 d . . .
Na1 Na -0.2649(6) -0.13877(12) -0.45721(18) 0.0237(6) Uani 1 1 d . . .
Na2 Na 0.2641(6) 0.18015(11) 0.03201(18) 0.0227(6) Uani 1 1 d . . .
Na3 Na 0.2376(6) -0.09973(12) -0.10507(18) 0.0244(6) Uani 1 1 d . . .
Na4 Na -0.7403(6) -0.05027(12) -0.47259(18) 0.0239(6) Uani 1 1 d . . .
Na5 Na 0.7396(6) 0.27056(12) 0.00744(19) 0.0257(6) Uani 1 1 d . . .
Na6 Na 0.7655(6) -0.01678(11) -0.07289(19) 0.0235(6) Uani 1 1 d . . .
O1 O -0.3903(10) 0.0523(2) -0.3552(3) 0.0213(10) Uani 1 1 d . . .
O2 O 0.8905(9) 0.2114(2) -0.3339(3) 0.0206(10) Uani 1 1 d . . .
O3 O -0.8926(10) 0.0145(2) -0.3598(3) 0.0218(10) Uani 1 1 d . . .
O4 O -0.2666(10) -0.0421(2) -0.4412(3) 0.0221(10) Uani 1 1 d . . .
O5 O -0.7288(11) 0.0710(2) -0.2238(3) 0.0253(11) Uani 1 1 d . . .
O6 O 0.2126(10) 0.1246(2) -0.3727(3) 0.0215(10) Uani 1 1 d . . .
O7 O 0.2714(10) 0.2782(2) 0.0476(3) 0.0201(10) Uani 1 1 d . . .
O8 O 0.1160(9) 0.1120(2) -0.0762(3) 0.0193(10) Uani 1 1 d . . .
O9 O -1.1192(10) -0.1455(2) -0.2979(3) 0.0220(11) Uani 1 1 d . . .
O10 O 0.3921(10) 0.2117(2) -0.2798(3) 0.0235(11) Uani 1 1 d . . .
O11 O -0.2612(10) -0.0392(2) -0.2650(3) 0.0230(11) Uani 1 1 d . . .
O12 O -0.6216(10) -0.1220(2) -0.2528(3) 0.0243(11) Uani 1 1 d . . .
O13 O -0.2426(10) -0.1091(2) -0.1328(3) 0.0211(10) Uani 1 1 d . . .
O14 O 0.6170(9) 0.0774(2) -0.0933(3) 0.0206(10) Uani 1 1 d . . .
O15 O 0.7363(10) 0.1738(2) -0.0072(3) 0.0208(10) Uani 1 1 d . . .
O16 O -0.7489(10) -0.14524(19) -0.4213(3) 0.0201(10) Uani 1 1 d . . .
O17 O 0.2387(10) 0.00032(19) -0.0838(3) 0.0210(10) Uani 1 1 d . . .
O18 O 0.7768(11) 0.1650(2) -0.1833(3) 0.0260(11) Uani 1 1 d . . .
O19 O -0.7496(11) -0.2257(2) -0.3032(3) 0.0280(12) Uani 1 1 d . . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Si1 O7 1.579(5) 4_565 ?
Si1 O10 1.621(5) . ?
Si1 O2 1.637(5) 1_455 ?
Si1 O6 1.641(5) . ?
Si1 Na1 3.091(3) 3_554 ?
Si1 Na5 3.140(3) 4_465 ?
Si1 Na2 3.390(3) 4_565 ?
Si1 Na5 3.425(4) 4_565 ?
Si2 O15 1.579(5) . ?
Si2 O18 1.616(5) . ?
Si2 O8 1.635(5) 1_655 ?
Si2 O14 1.648(5) . ?
Si2 Na2 3.098(3) 1_655 ?
Si2 Na3 3.106(3) 3_655 ?
Si2 Na2 3.406(4) . ?
Si2 Na5 3.512(3) . ?
Si3 O4 1.573(5) . ?
Si3 O11 1.621(5) . ?
Si3 O3 1.630(5) 1_655 ?
Si3 O1 1.646(5) . ?
Si3 Na4 2.963(3) 3_454 ?
Si3 Na4 3.091(4) 1_655 ?
Si3 Na4 3.319(3) . ?
Si3 Na1 3.479(3) . ?
Si4 O16 1.573(5) . ?
Si4 O19 1.625(5) . ?
Si4 O9 1.629(5) . ?
Si4 O12 1.638(5) . ?
Si4 Na1 3.101(3) 1_455 ?
Si4 Na5 3.309(3) 2_544 ?
Si4 Na1 3.389(4) . ?
Si4 Na4 3.448(3) . ?
Si5 O5 1.584(5) . ?
Si5 O6 1.608(5) 1_455 ?
Si5 O1 1.616(5) . ?
Si5 O3 1.623(5) . ?
Si6 O17 1.581(5) . ?
Si6 O5 1.614(5) 1_655 ?
Si6 O14 1.638(5) . ?
Si6 O8 1.640(5) . ?
Si6 Na6 3.014(3) . ?
Si6 Na6 3.175(3) 3_655 ?
Si6 Na6 3.299(3) 1_455 ?
Si7 O19 1.591(5) 2_554 ?
Si7 O18 1.598(5) . ?
Si7 O10 1.608(5) . ?
Si7 O2 1.616(5) . ?
Si8 O13 1.585(5) . ?
Si8 O11 1.632(5) . ?
Si8 O9 1.637(5) 1_655 ?
Si8 O12 1.639(5) . ?
Si8 Na3 3.009(4) 1_455 ?
Si8 Na6 3.248(3) 1_455 ?
Si8 Na3 3.307(3) . ?
Na1 O4 2.284(6) . ?
Na1 O7 2.395(5) 2_544 ?
Na1 O16 2.443(6) . ?
Na1 O9 2.558(5) 1_655 ?
Na1 O16 2.593(5) 1_655 ?
Na1 O6 2.651(6) 3_554 ?
Na1 Si1 3.091(3) 3_554 ?
Na1 Si4 3.101(3) 1_655 ?
Na1 Na4 3.132(4) . ?
Na1 Na5 3.247(4) 2_544 ?
Na1 Na4 3.316(4) 1_655 ?
Na2 O13 2.282(6) 3 ?
Na2 O7 2.315(5) . ?
Na2 O15 2.400(6) . ?
Na2 O8 2.420(5) . ?
Na2 O15 2.660(5) 1_455 ?
Na2 Si2 3.098(3) 1_455 ?
Na2 Na5 3.177(4) . ?
Na2 Na3 3.285(4) 3_655 ?
Na2 Na3 3.301(4) 3 ?
Na2 Na5 3.355(4) 1_455 ?
Na2 Si1 3.390(3) 4_566 ?
Na3 O17 2.372(5) . ?
Na3 O13 2.402(5) . ?
Na3 O12 2.434(6) 1_655 ?
Na3 O15 2.456(6) 3_655 ?
Na3 O13 2.595(6) 1_655 ?
Na3 Si8 3.009(4) 1_655 ?
Na3 Na6 3.067(4) 1_455 ?
Na3 Si2 3.106(3) 3_655 ?
Na3 Na6 3.276(4) . ?
Na3 Na2 3.285(4) 3_655 ?
Na3 Na2 3.301(4) 3 ?
Na4 O16 2.366(5) . ?
Na4 O4 2.379(5) . ?
Na4 O3 2.427(6) . ?
Na4 O4 2.542(6) 3_454 ?
Na4 O4 2.634(6) 1_455 ?
Na4 O1 2.728(6) 3_454 ?
Na4 Si3 2.963(3) 3_454 ?
Na4 Si3 3.091(4) 1_455 ?
Na4 Na1 3.316(4) 1_455 ?
Na4 Na4 3.442(6) 3_454 ?
Na5 O15 2.283(5) . ?
Na5 O16 2.381(5) 2_554 ?
Na5 O7 2.386(6) . ?
Na5 O2 2.584(5) 4_566 ?
Na5 O7 2.685(5) 1_655 ?
Na5 Si1 3.140(3) 4_666 ?
Na5 Na1 3.247(4) 2_554 ?
Na5 Si4 3.309(3) 2_554 ?
Na5 Na2 3.355(4) 1_655 ?
Na5 Si1 3.425(4) 4_566 ?
Na5 Na1 3.432(4) 2_654 ?
Na6 O14 2.350(5) . ?
Na6 O13 2.355(5) 1_655 ?
Na6 O17 2.361(6) 1_655 ?
Na6 O17 2.442(6) 3_655 ?
Na6 O17 2.619(6) . ?
Na6 O11 3.005(6) 1_655 ?
Na6 Na3 3.067(4) 1_655 ?
Na6 Si6 3.175(3) 3_655 ?
Na6 Si8 3.248(3) 1_655 ?
Na6 Si6 3.299(3) 1_655 ?
O1 Na4 2.728(6) 3_454 ?
O2 Si1 1.637(5) 1_655 ?
O2 Na5 2.584(5) 4_565 ?
O3 Si3 1.630(5) 1_455 ?
O4 Na4 2.542(6) 3_454 ?
O4 Na4 2.634(6) 1_655 ?
O5 Si6 1.614(5) 1_455 ?
O6 Si5 1.608(5) 1_655 ?
O6 Na1 2.651(6) 3_554 ?
O7 Si1 1.579(5) 4_566 ?
O7 Na1 2.395(5) 2_554 ?
O7 Na5 2.685(5) 1_455 ?
O8 Si2 1.635(5) 1_455 ?
O9 Si8 1.637(5) 1_455 ?
O9 Na1 2.558(5) 1_455 ?
O11 Na6 3.005(6) 1_455 ?
O12 Na3 2.434(6) 1_455 ?
O13 Na2 2.282(6) 3 ?
O13 Na6 2.355(5) 1_455 ?
O13 Na3 2.595(6) 1_455 ?
O15 Na3 2.456(6) 3_655 ?
O15 Na2 2.660(5) 1_655 ?
O16 Na5 2.381(5) 2_544 ?
O16 Na1 2.593(5) 1_455 ?
O17 Na6 2.361(6) 1_455 ?
O17 Na6 2.442(6) 3_655 ?
O19 Si7 1.591(5) 2_544 ?
